Download Presentation

Loading in 3 Seconds

This presentation is the property of its rightful owner.

X

Sponsored Links

- 288 Views
- Uploaded on
- Presentation posted in: General

Calculations of Hyperfine parameters in solids based on DFT and using WIEN2k

Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.

- - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - -

Calculations of Hyperfine parameters in solids based on DFT and using WIEN2k

Peter Blaha

Institute of Materials Chemistry

TU Wien

- Isomer shift: d = a (r0Sample – r0Reference);
- it is proportional to the electron density r0at the nucleus
- the constant a is proportional to the change of nuclear radii during the transition (we use a=-.291 au3mm s-1)

- Magnetic Hyperfine fields: Btot = Bcontact + Borb + Bdip
- these fields are proportional to the spin-density at the nucleus and the orbital moment of the probed atom as well as the spin moment distribution in the crystal

- Quadrupole splitting: De Q Vzz
- given by the product of the nuclear quadrupole moment Q times the electric field gradient Vzz. The EFG is proportional to an integral over the non-spherical charge density (weighted by 1/r3)

- From the previous slide it is obvious, that we need an accurate knowledge of the electron (and magnetization) density, which in principle can be obtained from the solution of the many-body Schrödinger equation for the corresponding solid.
H Y = E Y

- However, a many-body problem with ~1023 particles is not solvable at all and we must create models for the real material and rely on an approximate solution of the Schrödinger equation. (This will be briefly discussed in the next slides and my preferred options are marked in red.)

- Representation of the solid:
- cluster model: approximate solid by a finite cluster
- periodic model: approximate “real” solid by infinite ideal solid
- (supercells !)

BaSnO3

If calculations disagree with

experiment:

the structural model could be wrong

- Exchange and correlation:
- Hartree-Fock (exact exchange, no correlation)
- correlation: MP2, CC, ...

- Density functional theory: approximate exchange + correlation
- LDA: local density approximation, “free electron gas”
- GGA: generalized gradient approximation, various functionals
- hybrid-DFT: mixing of HF + GGA, various functionals
- LDA+U, DMFT: explicit (heuristic) inclusion of correlations

- Hartree-Fock (exact exchange, no correlation)

If calculations disagree with experiment:

the DFT approximation could be too crude

- basis set for wavefunctions:
- “quantum chemistry”: LCAO methods
- Gauss functions (large “experience”, wrong asymptotics, ... )
- Slater orbitals (correct r~0 and r~ asymptotics, expensive)
- numerical atomic orbitals

- “physics”: plane wave based methods
- plane waves (+ pseudopotential approximation)
- augmented plane wave methods (APW)
- combination of PW (unbiased+flexible in interstitial regions)
- + numerical basis functions (accurate in atomic regions, cusp)

- “quantum chemistry”: LCAO methods

- Computational approximations:
- relativistic treatment:
- non-, scalar-, fully-relativistic treatment

- treatment of spin, magnetic order
- approximations to the form of the potential
- shape approximations (ASA)
- pseudopotential (nodeless valence orbitals)
- “full potential”

- relativistic treatment:

- in many cases, the experimental knowledge about a certain system is very limited and also the exact atomic positions may not be known accurately (powder samples, impurities, surfaces, ...)
- Thus we need a theoretical method which can not only calculate HFF-parameters, but can also model the system:
- total energies + forces on the atoms:
- perform structure optimization for “real” systems
- calculate phonons (+ partial phonon-DOS)
- investigate various magnetic structures, exchange interactions

- electronic structure:
- bandstructure + DOS
- compare with ARPES, XANES, XES, EELS, ...

- hyperfine parameters
- isomer shifts, hyperfine fields, electric field gradients

- total energies + forces on the atoms:

An Augmented Plane Wave Plus Local Orbital

Program for Calculating Crystal Properties

Peter Blaha

Karlheinz Schwarz

Georg Madsen

Dieter Kvasnicka

Joachim Luitz

November 2001

Vienna, AUSTRIA

Vienna University of Technology

WIEN2k: ~1700 groups

mailinglist: 1800 users

http://www.wien2k.at

- The unit cell is partitioned into:
- atomic spheres
- Interstitial region

unit cell

Rmt

ul(r,e) are the numerical solutions

of the radial Schrödinger equation

in a given spherical potential for a

particular energy e

AlmKcoefficients for matching the PW

Basisset:

PW:

join

Atomic partial waves

“Exact” solution for given (spherical) potential!

- Structure generator
- spacegroup selection
- import cif file

- step by step initialization
- symmetry detection
- automatic input generation

- SCF calculations
- Magnetism (spin-polarization)
- Spin-orbit coupling
- Forces (automatic geometry optimization)

- Guided Tasks
- Energy band structure
- DOS
- Electron density
- X-ray spectra
- Optics

- The coulomb potential Vcis a central quantity in any theoretical calculation
- (part of the Hamiltonian) and is obtained from all charges r (electronic +
- nuclear) in the system.
- The EFG is a tensor of second derivatives of VC at the nucleus:
- Since we use an “all-electron” method, we have the full charge distribution
- of all electrons+nuclei and can obtain the EFG without further approximations.
- The spherical harmonics Y20 projects out the non-spherical (and non-cubic)
- part of r. The EFG is proportional to the differences in orbital occupations
- (eg. pz vs. px,py)
- We do not need any “Sternheimer factors”
- (these shielding effects are included in the self-consistent charge density)

- The charge density r in the integral can be decomposed in various ways for analysis:
- according to energy (into various valence or semi-core
contributions)

- according to angular momentum l and m (orbitals)
- spatial decomposition into “atomic spheres” and the “rest” (interstital)

- according to energy (into various valence or semi-core
- Due to the 1/r3 factor, contributions near the nucleus dominate.

EF

We write the charge density and the potential inside the atomic spheres in an lattice-harmonics expansion

interstitial

- EFG is proportial to differences of orbital occupations ,
- e.g. between px,py and pz.
- if these occupancies are the same by symmetry (cubic): Vzz=0
- with “axial” (hexagonal, tetragonal) symmetry (px=py): h=0
- In the following various examples will be presented.

Compare theoretical and experimental EFGs Q

( previous value)

FeF2

FeSi

FeZr3

Fe2O3

FeNi

YFe2

Fe2P

FeS2

Fe4N

FeCl2

FeBr2

(exp.)

Isolated octahedra

Rings formed by four octahedra sharing corners

Isolated chains of octahedra linked by corners

a-BaAlF5

a-BaCaAlF7

Ba3Al2F12

F - EFGs in fluoroaluminates

10 different phases of known structures from CaF2-AlF3,

BaF2-AlF3 binary systems and CaF2-BaF2-AlF3 ternary system

a-CaAlF5, b-CaAlF5,

b-BaAlF5, g-BaAlF5

Ca2AlF7, Ba3AlF9-Ib,

b-Ba3AlF9

hQ,exp= 0,803hQ,calR2 = 0,38

nQ= 4,712.10-16 |Vzz| with R2 = 0,77

Important discrepancies when structures are used which were determined from X-ray powder diffraction data

nQ and hQcalculations using XRD data

Attributions performed with respect to the proportionality between |Vzz| and nQfor the multi-site compounds

nQ = 5,85.10-16 Vzz R2 = 0,993

hQ, exp = 0,972hQ,cal

R2 = 0,983

nQand hQafter structure optimization

Very fine agreement between experimental and calculated values

- M.Body, et al., J.Phys.Chem. A 2007, 111, 11873 (Univ. LeMans)

- The earth lower mantle consists of (Mg,Fe)O and
- (Mg1-xFex)SiO3 perovskite

(Mg,Fe)

Mössbauerunder pressure (McCammon)

QS: 2.4 mm/s

QS: 3.5 mm/s

interpretation:

high-spin intermediate spin transition

HS (M=4uB) IS (M=2uB) LS (M=0)

eg

t2g

eg

t2g

crystal field: small intermediate large

spin splitting: large intermediate zero t2g

- extensive structure optimizations (including soft phonons) of various possible spin states at different pressures and with different orbital occupations:
- leading to several (meta-) stable phases:

P (GPa)

- two different HS states compete with each other
- IS state never the ground state
- LS state not stable at relevant pressures

electronicHS - HS transition

spin-dn e-: dyzdxy+dx2-y2

H. Hsu et al., Earth and Planetary Science Letters 294 (2010) 19–26

(temperature induced PT between charge-ordered and mixed valence state)

2 Fe2.5+ Fe2+ + Fe3+

ABO3 O-deficient double-perovskite

Ba

Y (R)

square pyramidal

coordination

Antiferromagnet with a 2 step Verwey transition around 300 K

Woodward&Karen, Inorganic Chemistry 42, 1121 (2003)

CO structure: Pmma VM structure: Pmmm

a:b:c=2.09:1:1.96 (20K) a:b:c=1.003:1:1.93 (340K)

- Fe2+ and Fe3+ chains along b
- contradicts Anderson charge-ordering conditions with minimal electrostatic repulsion (checkerboard like pattern)
- has to be compensated by orbital ordering and e--lattice coupling

c

b

a

- Metallic behaviour/No bandgap
- Fe-dn t2g states not splitted at EF
- overestimated covalency between O-p and Fe-eg

- Magnetic moments too small
- Experiment:
- CO: 4.15/3.65 (for Tb), 3.82 (av. for Y)
- VM: ~3.90

- Calculation:
- CO: 3.37/3.02
- VM: 3.34

- Experiment:
- no significant charge order
- charges of Fe2+ and Fe3+ sites nearly identical

- CO phase less stable than VM
- LDA/GGA NOT suited for this compound!

Fe-eg t2g eg*t2g eg

- Hybrid-DFT
- ExcPBE0 [r] = ExcPBE [r] + a (ExHF[Fsel] – ExPBE[rsel])

- ELDA+U(r,n) = ELDA(r) + Eorb(n) – EDCC(r)
- separate electrons into “itinerant” (LDA) and localized e-(TM-3d, RE 4f e-)
- treat them with “approximate screened Hartree-Fock”
- correct for “double counting”

- Hubbard-U describes coulomb energy for 2e- at the same site
- orbital dependent potential

GGA+U GGA

single lower Hubbard-band in VM splits in CO with Fe3+ states lower than Fe2+

insulator, t2g band splits metallic

GGA+U

insulator metal

- Fe2+ (3d6) CO Fe3+ (3d5) VM Fe2.5+ (3d5.5)
- majority-spin fully occupied
- strong covalency effects very localized states at lower energy than Fe2+
in eg and d-xz orbitals

- minority-spin states
- d-xz fully occupied (localized) empty d-z2 partly occupied
- short bond in y short bond in z (one O missing) FM Fe-Fe; distances in z ??

- CO phase VM phase

Fe2+: d-xz

Fe3+: d-x2

O1 and O3: polarized

toward Fe3+

Fe: d-z2 Fe-Fe interaction

O: symmetric

- Fe3+: no contribution
- Fe2+: dxz
- weak p-bond with O
- tilting of O3 p-orbital

- Isomer shift: d = a (r0Sample – r0Reference); a=-.291 au3mm s-1
- proportional to the electron density r at the nucleus

- Magnetic Hyperfine fields: Btot=Bcontact + Borb + Bdip
- Bcontact = 8p/3 mB [rup(0) – rdn(0)] … spin-density at the nucleus
… orbital-moment

… spin-moment

- Bcontact = 8p/3 mB [rup(0) – rdn(0)] … spin-density at the nucleus

S(r) is reciprocal of the relativistic mass enhancement

Hyperfine fields: Fe2+ has large Borb and Bdip

Isomer shift: charge transfer too small in LDA/GGA

EFG: Fe2+ has too small anisotropy in LDA/GGA

CO

VM

- EFGs can routinely be calculated for all kinds of solids.
- “semi-core” contribution large for “left”-atoms of the periodic table
- p-p contribution always large (on-site (eg. O-2p) vs. off-site (Fe-4p))
- d-d (f-f) contributions for TM (lanthanide/actinide) compounds
- EFG stems from different orbital occupations due to covalency or crystal field effects

- EFG is very sensitive to
- correct structural data (internal atomic positions)
- correct theoretical description of the electronic structure
- “highly correlated” transition metal compounds (oxides, halides)
- 4f and 5f compounds
- “beyond” LDA (LDA+U, Hybrid-DFT, …)

K.Schwarz, C.Spiel, R.Laskowski, TU Vienna

Han Hsu, R. Wentzcovitch, Univ. Minnesota (perovskite)

M.Body, G.Silly, Univ. Le Mans (Al-fluorides)

Thank you for

your attention !

- above TN (~430 K): tetragonal (P4/mmm)
- 430K: slight orthorhombic distortion (Pmmm) due to AFM
- all Fe in class-III mixed valence state +2.5;
- ~334K: dynamic charge order transition into class-II MV state,
- visible in calorimetry and
- Mössbauer, but not with X-rays
- 308K: complete charge order into
- class-I MV state (Fe2+ + Fe3+)
- large structural changes (Pmma)
- due to Jahn-Teller distortion;
- change of magnetic ordering:
- direct AFM Fe-Fe coupling vs.
- FM Fe-Fe exchange above TV

CO phase: G-type AFMVM phase:

- AFM arrangement in all directions, AFM for all Fe-O-Fe superexchange paths
also across Y-layer FM across Y-layer (direct Fe-Fe exchange)

- Fe moments in b-direction

4 8

independent Fe atoms

- magnetic moments in very good agreement with exp.
- LDA/GGA: CO: 3.37/3.02 VM: 3.34 mB
- orbital moments small (but significant for Fe2+)

- exp: semiconductor (like Ge); VM phase has increased conductivity
- LDA/GGA: metallic

- Charges according to Baders “Atoms in Molecules” theory
- Define an “atom” as region within a zero flux surface
- Integrate charge inside this region

O2a

- CO phase:
- Fe2+:shortest bond in y (O2b)
- Fe3+: shortest bond in z (O1)

- VM phase:
- all Fe-O distances similar
- theory deviates along z !!
- Fe-Fe interaction
- different U ??
- finite temp. ??

O2b

O3

O1

O1

- Take Ueff as “empirical” parameter (fit to experiment)
- Estimate Ueff from constraint LDA calculations
- constrain the occupation of certain states (add/subtract e-)
- switch off any hybridization of these states (“core”-states)
- calculate the resulting Etot
- we used Ueff=7eV for all calculations

- CO phase:
- magneto-crystalline anisotropy:
moments point into y-direction

in agreement with exp.

- experimental G-type AFM structure (AFM direct Fe-Fe exchange) is 8.6 meV/f.u. more stable than magnetic order
of VM phase (direct FM)

- magneto-crystalline anisotropy:
- VM phase:
- experimental “FM across Y-layer”
AFM structure (FM direct Fe-Fe exchange)

is 24 meV/f.u. more stable than magnetic

order of CO phase (G-type AFM)

- experimental “FM across Y-layer”

- Heisenberg model: H = Si,j JijSi.Sj
- 4 different super-exchange interactions (Fe-Fe exchange interaction mediated by an O atom)
- J22b : Fe2+-Fe2+ along b
- J33b : Fe3+-Fe3+ along b
- J23c : Fe2+-Fe3+ along c
- J23a : Fe2+-Fe3+ along a

- 1 direct Fe-Fe interaction
- Jdirect: Fe2+-Fe3+ along c
- Jdirect negative (AFM) in CO phase
- Jdirect positive (FM) in VM phase

- S.Chang etal., PRL 99, 037202 (2007)
- J33b = 5.9 meV
- J22b = 3.4 meV
- J23 = 6.0 meV
- J23 = (2J23a + J23c)/3

- Total energy of a certain magnetic configuration given by:
ni … number of atoms i

zij … number of atoms j which

are neighbors of i

Si = 5/2 (Fe3+); 2 (Fe2+)

si = ±1

- Calculate E-diff when a spin on atom i (Di) or on two atoms i,j (Dij) are flipped
- Calculate a series of magnetic configurations and determine Jij by least-squares fit

- Standard LDA/GGA methods cannot explain YBaFe2O5
- metallic, no charge order (Fe2+-Fe3+), too small moments

- Needs proper description of the Fe 3d electrons (GGA+U, …)
- CO-phase: Fe2+: high-spin d6, occupation of a single spin-dn orbital (dxz)
- Fe2+/Fe3+ ordered in chains along b, cooperative Jahn-Teller distortion and strong e--lattice coupling which dominates simple Coulomb arguments (checkerboard structure of Fe2+/Fe3+)

- VM phase: small orthorhombic distortion (AFM order, moments along b)
- Fe d-z2 spin-dn orbital partly occupied (top of the valence bands)
leads to direct Fe-Fe exchange across Y-layer and thus to ferromagnetic order (AFM in CO phase).

- Fe d-z2 spin-dn orbital partly occupied (top of the valence bands)
- Quantitative interpretation of the Mössbauer data
- Calculated exchange parameters Jij in reasonable agreement with exp.